O R I G I N A L A R T I C L E
Solute diffusion into cell walls in solution-impregnated wood
under conditioning process I: effect of relative humidity on solute
Soichi Tanaka1,2•Masako Seki3•Tsunehisa Miki3•Ichinori Shigematsu3•
Received: 4 February 2015 / Accepted: 16 July 2015 / Published online: 3 September 2015 The Japan Wood Research Society 2015
Abstract This study focused on solute diffusing into cell walls in solution-impregnated wood under conditioning. The purpose of this paper was to clarify the effect of rel-ative humidity (RH) of the conditioning on solute diffu-sivity in the impregnated wood. Water evaporation, swelling, and shrinkage of wood samples impregnated with an aqueous solution of polyethylene glycol (PEG) polymer were examined under conditioning at an RH of 11, 32, 55, or 80 % followed by drying under vacuum. Dried samples were observed using a micro-focus X-ray computed tomography instrument. The total amount of PEG polymer diffusing into cell walls during conditioning increased with RH. Theoretical interpretation indicated that this was caused by an increase in polymer (solute) diffusivity as the amount of water (solvent) in samples increased. Temporal variability of the evaporation rate of water and of the swelling rate of the sample also were examined. Solute diffusivity, which was similar at each RH at the beginning of conditioning, decreased during conditioning; this decrease was greater at lower RH values due to a higher evaporation rate.
Keywords Impregnated woodConditioning Relative humiditySolute diffusivitySolvent evaporation
Treatment of wood with a non-volatile substance has been used to overcome the disadvantages of wood, such as a lack of homogeneity, its tendency to deform in water and moist air, and its ability to be degraded by sunlight, fungi, and insects. Wood properties are well known to be improved, to some extent, by treatment with an appropriate substance (for example, ). The method of treatment, however, has not been well studied. Several studies have shown that the amount of a substance in wood cell walls mainly deter-mines the wood properties such as dimensional stability (for example, ). Thus, filling up cell walls with a sub-stance is necessary for the efficient treatment.
Treatment processes include impregnation and condi-tioning (Fig.1a). For impregnation, the wood is soaked in a solution of a non-volatile substance (solute), and then placed under a vacuum (or subjected to pressure) while in contact with the treatment solution. For conditioning, the impregnated wood is placed under an atmosphere. For both processes, migration of solute and solvent occurs at a cellular level (Fig.1b):
• During impregnation, the solution uniformly permeates the cell walls and cell cavities.
• During conditioning, a greater amount of solvent evaporates from the cell cavities than from the cell walls, which increases the concentration of solute in the cavities than that in the walls. This concentration difference causes diffusion of the solute from the cavities to the walls .
Part of this report was presented at the 64th Annual Meeting of the Japan Wood Research Society, Matsuyama, March 2014.
& Soichi Tanaka
1 Research Institute for Sustainable Humanosphere, Kyoto University, Gokasho, Uji, Kyoto 611-0011, Japan 2 Formerly Materials Research Institute for Sustainable
Development, National Institute of Advanced Industrial Science and Technology, Moriyama-ku, Nagoya, Aichi 463-8560, Japan
3 Structural Materials Research Institute, National Institute of Advanced Industrial Science and Technology, Moriyama-ku, Nagoya, Aichi 463-8560, Japan
The solute permeability during impregnation has been studied by many researchers using polyethylene glycol (PEG) polymer as a solute [3–14]. Jeremic et al.  examined the effect of nature of solvent on amount of the polymers in cell walls and estimated the diffusion rate of the polymers into cell walls . Tarkow et al.  examined the effect of the molecular size on amount of the polymers penetrated into wood. Stamm [12, 13] investigated a variety of factors that affect amount of the polymers in call walls and cell cavities during impregna-tion. Stamm  also proposed the mechanism of solute diffusing into cell walls during conditioning. This mech-anism has, however, never been verified. Solute amount in the cell walls will increase if the solute diffusion is pro-moted during the conditioning, while the amount will not increase if the diffusion is not promoted (Fig.1b). Therefore, there exists the possibility of maximizing the solute amount in the cell walls in short time by optimizing the conditioning.
The objective of this study is to determine the conditions that maximize amount of solute diffusing into the cell walls of solution-impregnated wood during the conditioning process in short time. Amount of solute diffusing into cell walls is determined by:
• Concentration difference of the solute between the cell walls and cell cavities.
• Solute diffusivity.
These two factors are affected mainly by solution condi-tions (such as concentration and type of solute and solvent), material conditions (such as wood species and dimension), and atmospheric conditions (such as temperature and vapor pressure of the solvent). Control of the atmospheric con-ditions is necessary since the other concon-ditions often depend on the demanded properties of the treated wood. Solvent vapor pressure is especially important, because it is easily controlled for determining its effect on solution-impreg-nated wood.
Fig. 1 aProcess and
Relative humidity (RH) is often used as an indicator of solvent vapor pressure, because water is used often as a solvent due to its high affinity toward wood. In our previous studies [15,16], the effect of RH on the concentration dif-ference was determined, but the effect on solute diffusivity could not be evaluated by investigating the swelling and shrinkage behavior of wood impregnated with an aqueous solution of PEG during conditioning at high RH values (close to the saturated vapor pressure). Solute diffusivity was expected to experience greater change within the lower RH range where the cell walls contain less bound water, on the basis of the fact that diffusion of the polymers into cell walls is much more rapid if moisture is present in wood .
The purpose of this paper was to clarify the effect of RH on the solute diffusivity. Water evaporation and the swel-ling-shrinkage behavior of wood impregnated with an aqueous solution of PEG polymers were examined during conditioning at several RHs including the lower RHs. Conditioned wood was dried under vacuum and its mass and dimension were measured. A cross section of a dried sample was observed using a micro-focus X-ray computed tomography (CT) system. The effect of RH on the polymer diffusivity was interpreted based on theoretical factors. Temporal variability in the water evaporation rate and swelling rate were examined in terms of solute diffusivity.
Effect of RH on solute diffusivity could not be directly observed. Therefore, the relation between RH and amount of solute diffusing into cell walls, which could be estimated using dimension of sample, was qualitatively predicted by the model of substance migration (Fig.2) considering the solute diffusivity. The process of the prediction is shown as follows.
Solvent evaporated from the samples can be separated into those from the cell cavities and from the cell walls. The amount of solvent evaporated from the cell cavities and cell walls, -DnC0 and -DnW0, respectively, can be
for-mulated as :
DnC0¼KðPSPAPCÞDt; ð1Þ DnW0¼KðPSPAPWÞDt; ð2Þ
whereKrepresents surface evaporation coefficient ([0),PS
is saturated vapor pressure of the solvent, PA is vapor
pressure of the solvent in the atmosphere,PC andPWare
evaporation resistance pressure on the boundary between the atmosphere and the wood elements (cell cavity and cell wall, respectively).
The relation PS -PA=PW=PC exists immediately
before the conditioning. In the unsteady state during condi-tioning, the inequality ofPS-PA[PW[PC[0 exists,
because vapor pressure decreases to a level corresponding to RH, and water retentivity of the cell wall is higher than that of the cell cavity due to higher energy to remove bound water from the cell wall . From this inequality, and Eqs. (1) and (2), the following expression can be deduced:
This inequality indicates that more solvent evaporates from the cell cavities than from the cell walls.
Causal relations among solute diffusion, solute concentration difference, and solvent evaporation
The amount of solute diffusing into cell walls during infinitesimal timeDtcan be expressed as:
whereK1is solute diffusivity ([0), and xC1 andxW1
rep-resent molar fractions of solute in the cell cavity and cell wall, respectively.
The solute concentration difference between the cell walls and cell cavities changes as solvent evaporates from the wood. Immediately before conditioning, the difference is absent producing the following equation:
wherenC0andnW0represent moles of solvent in cell cavity
and cell wall, respectively,nC1andnW1are moles of solute
in the cell cavity and cell wall, respectively,nWis number
in moles of sorption sites of solution in the cell wall. The concentration difference changes with time (Dt) after the start of conditioning [Eq. (6)]; the inequality relation of Eq. (6) was deduced from Eq. (3).
The inequality indicates that a solute concentration in the cell cavities greater than that in the cell walls is caused by solvent evaporation. The inequality DnW1[0 is deduced
from Eqs. (4) and (6), which indicates that the solute dif-fuses from the cell cavities to the cell walls due to the concentration difference.
Relation between RH and total amount of solute diffusing during conditioning
The solute diffusivity,K1, was assumed in this paper to
increase with the amount of solvent in the sample. If it was also assumed that the amount of solvent (water) in the sample increases with RH during conditioning (Fig.3b), the value ofK1also increases with RH (gray dotted line in
The solute concentration difference, xC1-xW1,
increases as RH orPA(Fig.2) decreases (gray broken line
in Fig.3a), because DnC0andDnW0, which have negative
values, decrease withPA [Eqs. (1) and (2)], and because
the value of xC1-xW1 increases as DnC0 and DnW0
decreases [Eq. (6)]. This tendency was also supported by our previous study .
The concave-downward curve showing the relation of the amount of solute diffusing duringDtto RH (gray solid line in Fig.3a) can be deduced by Eq. (4), and the relations ofK1andxC1-xW1to RH (see ‘‘Appendix’’ section). The
total amount of solute diffusing during conditioning was the time integration of the amount of solute diffusing during Dt. Thus, the relation of the total amount to RH (black line in Fig.3a) was approximately the same shape as the relation duringDt.
Materials and methods
Twelve cross-cut-wood samples, with dimensions of 5 mm925 mm925 mm in longitudinal (L), radial (R), and tangential (T) directions, respectively, were subse-quently prepared from a block of hinoki (Chamaecyparis
obtusa). The samples were dried at 105C to relatively
constant mass, followed by measurement of their width in the T direction.
The oven-dried samples were soaked in a 30 mass % aqueous solution of polyethylene glycol with an average molecular weight of 1500 (PEG1540, E.P., Wako), placed under vacuum at 0.01 MPa in 1 h, and then subjected to pressure at 0.8 MPa in 20 h in an impregnation plant (YA-10, Yasujima). The samples then were placed in the solu-tion at ambient pressure for 1 week.
The impregnated samples were blotted and their T width was measured. The samples were divided equally into four groups and conditioned for 900 h in a desiccator (MD-1, Sanplatec) at an RH of 11, 32, 55, or 80 % and temperature of 35C using supersaturated solutions of lithium chloride (LiCl), magnesium chloride (MgCl2), sodium bromide
Fig. 2 Model of substance migrating in and around a sample during an infinitesimal time,Dt.PS, saturated vapor pressure of solvent;PA, vapor pressure of solvent in the atmosphere;PCandPW, evaporation resistance pressure on the boundary between the atmosphere and wood elements (cell cavity and cell wall, respectively);K, surface evaporation coefficient;nC0andnW0, moles of solvent in cell cavity
(NaBr), or potassium bromide (KBr), respectively . The mass and T width of the samples were monitored over 1–900 h of conditioning.
All of the conditioned samples were removed from the desiccator and dried to relatively constant mass and T width in a vacuum chamber (0.01 MPa) with phosphorus pentoxide (P2O5).
The moisture content and relative swelling of the impregnated samples during conditioning as a function of conditioning timet,M(t) andr(t), and the relative swelling after conditioned and subsequently dried in a vacuum,rV,
were defined as follows:
MðtÞ ¼100fmðtÞ mVg
rðtÞ ¼ wðtÞ w0
wherew0represents T width of the oven-dry sample before
impregnation, w(0) is T width of the impregnated sample just before conditioning (t=0),m(t) andw(t) are mass and T width, respectively, of the impregnated sample during conditioning as a function oft,mVandwVare mass and T
width, respectively, after conditioned and subsequently dried in a vacuum.
The evaporation rate and swelling rate of the impreg-nated samples during conditioning,-DM/DtandDr/Dt, as a function oft were defined as follows:
Dr Dt ¼
whereti(i=0, 1, 2,…) is the conditioning time when the
mass and width were measured (t0=0\t1\t2\).
A block with a dimension of 5 mm (L)98 mm (R)98 mm (T) was cut from the center of the sample that was conditioned at each RH and subsequently dried. The center of the block was scanned using a micro-focus X-ray CT system (SMX-160CT-SV3S, Shimadzu) [20, 21] to obtain a two-dimensional tomogram with a field of view size of 1.68 mm in both the R and T directions and with a pixel size and slice thickness of 3 and 18lm, respectively.
Results and discussion
Water evaporation and swelling-shrinkage
behaviors of impregnated wood under conditioning
Figure4a shows the temporal variability in moisture con-tent of the aqueous PEG-solution-impregnated sample during conditioning. The moisture content or amount of water in the sample increased with RH during conditioning, which satisfied the assumption (Fig.3b) in the theory.
Figure4b shows the temporal variability in relative swelling of an impregnated sample during conditioning. The samples shrunk over time at RH values of 11 and 32 %, while they swelled over time at RH values of 55 and 80 %. The relative swelling at the conditioning time of 900 h (equilibrium point) increased with RH. This swelling and shrinkage behavior was considered to be caused by the PEG polymers diffusing into the cell walls and by the water exuding from the cell walls, respectively . To evaluate the effect of RH on polymer diffusing into the cell walls, the effect of water on the dimensions of the samples had to be eliminated.
Effect of RH on polymer diffusivity
Figure5 shows the relation between RH and relative swelling of samples that were conditioned and subse-quently dried in a vacuum to eliminate the effect of water on the samples. During drying in vacuum, the amount of solute diffusing into cell walls was considered to be small. This is because the polymer with molecular weight higher than 400 lose its diffusivity if the sample is dried up  and because it generally takes shorter time to evaporate
water in drying in a vacuum than in the conditioning at RH=11 % at which the solute diffusion will be indicated in the latter description to be small. Thus, the relative swelling in Fig.5 is considered to show the amount of polymer migration into the cell walls. The amount of polymer diffusing into the cell walls during conditioning increased with RH, producing a concave-downward curve (Fig.5), which agrees with the theoretical trend (black solid line in Fig.3a). This agreement indicates that the theory was valid. On the basis of the theory, the tendency of the increase and decrease in the amount of the polymer diffusing into the cell walls with the RH is caused by the solute diffusivity and concentration difference, respectively (Fig.3a). Thus, it was indicated in the measured RH range (Fig.5) that the solute diffusivity affected the amount of the diffusing polymers much more than the concentration difference did. It was also indicated from the theory that the solute diffusivity was affected by the RH.
To confirm the polymer distribution in the samples that were conditioned and dried, the CT images of the RT cross section of the samples at each conditioning RH value were observed (Fig.6a–d). The cell cavities completely filled with the polymers in each image were counted by the visual observations. The number of the filled cavities showed a strong negative correlation with the relative swelling for the same samples as shown in Fig. 7. This indicates that the relative swelling increased with the polymer amount in the cell walls, because the non-volatile polymers did not evaporate from the samples during con-ditioning and drying processes. Thus, these findings sup-port the increase in polymer diffusing into cell walls during conditioning with RH.
Temporal variability of polymer diffusivity
Figure8a shows the temporal variability in evaporation rate, –DM/Dt, of water from impregnated samples during conditioning. The lower the RH, the greater the maximum value of evaporation rate, and the earlier the time until the evaporation rate reached zero.
Figure8b shows the temporal variability in swelling rate, Dr/Dt, during conditioning. The phase in which the sample swells, when the polymers diffuse into the cell walls, existed except at an RH of 11 %. The phase in which the specimen shrunk, when the water exudates from the cell walls, existed except at an RH of 80 %. Maximum swelling rate (Fig.8b) appeared after the maximum evap-oration rate (Fig.8a) and occurred earlier at lower RH values. This indicates a shorter time between the initiation of conditioning and polymer diffusion at lower RH values because of the larger concentration difference (gray broken line in Fig.3a) caused by the higher evaporation rate (Fig.8a). The slowest swelling rate (Fig.8b) occurred
Fig. 4 Temporal variability inamoisture content,M, andbrelative swelling, r, of impregnated samples during conditioning at each relative humidity (RH).Barsstandard deviations
earlier at lower RH values. This indicates that the polymer diffusivity, which was consistent at each RH value at the start of conditioning, decreased during conditioning; the decrease was greater at lower RH due to a higher evapo-ration rate.
bFig. 6 Tomogram of a RT cross section of the sample conditioned at each relative humidity (RH) and subsequently dried under vacuum
Fig. 7 Relation of relative swelling of samples conditioned and subsequently dried under vacuum,rV, to number of cell cavities filled with polymers in each image in Fig.6,N.Barsstandard deviations
Water evaporation and swelling and shrinkage of aqueous PEG-solution-impregnated wood samples were examined during conditioning at an RH value of 11, 32, 55, or 80 %, followed by drying under vacuum, and compared against theoretical prediction. The dried samples were observed using a micro-focus X-ray CT system. Results showed: 1. The total amount of PEG polymers diffusing into the cell
walls during conditioning increased with RH. Theoret-ical interpretation indicated that this trend was caused by an increase in the polymer (solute) diffusivity with the amount of water (solvent) in the samples.
2. Temporal variability in the evaporation rate of water and of the swelling rate of the samples indicated that solute diffusivity was consistent at each RH value at the start of conditioning but decreased during condi-tioning; the decrease was greater at lower RH due to a higher evaporation rate.
Thus, conditioning of wood impregnated with a solution is efficient for the treatment of wood with solute if solvent vapor pressure is appropriately controlled. To develop a successful conditioning schedule, temporal variability in RH remains to be optimized, and the effect of factors such as temperature and solution concentration on the solute diffusing into cell walls should be investigated.
Acknowledgments Observations of the samples using micro-focus X-ray CT system were conducted in the Graduate School of Agri-culture, Kyoto University. The authors would like to express their gratitude to Mr. Yosuke Matsuda, Dr. Yoshiyuki Yanase, and Dr. Yoshihisa Fujii in the University for their help.
The relation of the amount of solute diffusing during Dt, DnW1, to RH, H, was shown to be a concave-downward
curve as follows.
According to the assumption in theory,K1andxC1-xW1
were formulated as follows:
K1 ¼aH; ð12Þ
xC1xW1¼ bHþc; ð13Þ
whereaandbrepresent constant of proportionality andcis intercept (a[0,b[0,c[0). The reason for the absence of the intercept in Eq. (12) is that the polymer completely loses its diffusivity at H=0, which is supported by the fact that the PEG polymer with molecular weight higher than 400 do not swell dried wood . The relation of DnW1 toHcan be deduced by Eqs. (4), (12), and (13) as
DnW1¼ ðabH2þacHÞDt: ð14Þ
The slope of the curve,DnW1(H), can be deduced by taking
the derivative ofDnW1with respect toHas follows:
dHðDnW1Þ ¼ ð2abHþacÞDt: ð15Þ In the RH range of H\c/2b, d(DnW1)/dH[0 consists,
and therebyDnW1increases withH. In the range ofH[c/
2b, d(DnW1)/dH\0 consists, and therebyDnW1decreases
with the increase inH. Thus, the relation ofDnW1toHhas
1. Inoue M, Ogata S, Nishikawa M, Otsuka Y, Kawai S, Norimoto M (1993) Dimensional stability, mechanical properties, and color changes of low molecular weight melamine-formaldehyde resin impregnated wood (in Japanese). Mokuzai Gakkaishi 39:181–189 2. Furuno T, Goto T (1978) Structure of the interface between wood and synthetic polymer. XI. The role of polymer in the cell wall on the dimensional stability of wood polymer composite (WPC). Mokuzai Gakkaishi 24:287–293
3. Stamm AJ (1956) Dimensional stabilization of wood with car-bonwaxes. For Prod J 6:201–204
4. Ishimaru Y (1993) PEG To Mokuzai No Hanashi (in Japanese). Mokuzaihozon 19:204–218
5. Jeremic D, Cooper P, Heyd D (2007) PEG bulking of wood cell walls as affected by moisture content and nature of solvent. Wood Sci Technol 41:597–606
6. Jeremic D, Cooper P (2009) PEG quantification and examination of molecular weight distribution in wood cell walls. Wood Sci Technol 43:317–329
7. Jeremic D, Quijano-Solis C, Cooper P (2009) Diffusion rate of polyethylene glycol into cell walls of red pine following vacuum impregnation. Cellulose 16:339–348
8. Kitani Y, Ohsawa J, Nakato K (1970) Adsorption of polyethylene glycol on water-swollen wood versus molecular weight (in Japanese). Mokuzai Gakkaishi 16:326–333
9. Sadoh T, Hashihira M (1973) A note on the swelling of wood with polyethylene glycols (in Japanese). Bull Kyoto Univ For 45:227–237 10. Schneider VA (1969) Contribution on the dimensional stabi-lization of wood with polyethylene glycol—part 1: basic inves-tigation on the dimensional stabilization of wood with polyethylene glycol (in German). Holz Roh Werkst 27:209–224 11. Schneider VA (1970) Contribution on the dimensional stabi-lization of wood with polyethylene glycol—part 2: investigation of changes of wood properties by PEG impregnation and on the effectiveness of various impregnation processes (in German). Holz Roh Werkst 28:20–34
12. Stamm AJ (1959) The dimensional stability of wood. For Prod J 9:375–381
13. Stamm AJ (1964) Factors affecting the bulking and dimensional stabilization of wood with polyethylene glycols. For Prod J 14:403–408
14. Tarkow H, Feist WC, Southerland CF (1966) Interaction of wood with polymeric materials penetration versus molecular size. For Prod J 16:61–65
of wood by drying treatment at an appropriate relative humidity. In: Proceedings of the 9th conference on sustainable development of energy, water and environment systems, Venice-Istanbul, September 2014, No. 0144
16. Tanaka S, Miki T, Seki M, Shigematsu I, Kanayama K (2015) Mechanism verification of solute diffusion into cell walls in solution impregnated wood under conditioning process: effect of relative humidity on swelling and shrinkage behavior of wood impregnated with an aqueous solution of polyethylene glycol (in Japanese). J Soc Mater Sci Jpn 64:369–374
17. Ogura T (1951) Studies on the mechanisms of wood drying (3): on the evaporating rate of moistures in wood (in Japanese). Ringyoshikenjyohokoku 51:61–75
18. Skaar C (1988) Wood-water relations. Springer, Berlin, pp 198–199
19. Greenspan L (1977) Humidity fixed points of binary saturated aqueous solutions. J Res Natl Bur Stand Sect A Phys Chem 81A:89–96
20. Matsuda Y, Fujiwara Y, Fujii Y (2015) Observation of machined surface and subsurface structure of hinoki (Chamaecyparis
obtusa) produced in slow-speed orthogonal cutting using X-ray
computed tomography. J Wood Sci 61:128–135